Research Article  Open Access
Yingjun Jiang, Yu Zhang, Changqing Deng, Yong Yi, Tian Tian, Kejia Yuan, "HighTemperature Rutting Resistance of Inverted Asphalt Pavement Structure", Advances in Civil Engineering, vol. 2020, Article ID 1937508, 10 pages, 2020. https://doi.org/10.1155/2020/1937508
HighTemperature Rutting Resistance of Inverted Asphalt Pavement Structure
Abstract
To improve the hightemperature rutting resistance of asphalt pavements, an inverted asphalt pavement structure (IAPS), 4 cm AC13 mixture + 8 cm AC25 mixture + 6 cm AC20 mixture + 54 cm cementstabilized macadam, was proposed herein by considering engineering practice, theoretical calculation, and analysis. A rutting prediction equation of asphalt pavements was then proposed via rutdevelopment trends found by laboratory 18 cm thick rutting test. Subsequently, the rutting resistance of the IAPS was evaluated. The results show that, compared with the traditional asphalt pavement structure (TAPS), 4 cm AC13 mixture + 6 cm AC20 mixture + 8 cm AC25 mixture + 54 cm cementstabilized macadam, the maximum shear stress of the IAPS can be reduced by ∼1.7% along with improvements in rutting resistance by ∼16% and ∼12% under wheel loads of 0.7 and 1.2 MPa, respectively. Wheelload increase affects the rutting resistance of both structures in a similar manner: when the wheel load increases from 0.7 MPa to 1.2 MPa, the rut depths of both pavement structures increase by at least 63%. The IAPS clearly has better rutting resistance than the TAPS and is thus the better choice for asphalt pavement structure design.
1. Introduction
Asphalt pavements offer advantages such as a flat surface, comfortable driving, low noise, fast construction, and simple maintenance and repairs. Therefore, they are widely used for paving roads all over the world [1,2]. However, as global temperatures continue to rise and as heavyduty and channelized traffic become increasingly commonplace, the usage conditions of asphalt pavements have become increasingly demanding, resulting in the reduced service life of typical asphalt pavements. Nowadays, insufficient durability has become the primary problem associated with the usage of asphalt pavements [3], often caused by pavement rutting [4,5].
Road engineers throughout the world have investigated various strategies for improving the asphalt pavement’s resistance to rutting at high temperatures [5–27]. Additives such as styrenebutalenestyrene (SBS) [6], ethylene copolymer [7], epoxy resin [8], rock asphalt [9], nanoparticles [10], highmodulus modifier [11], crumb rubber [12], and antirutting additives [13] have been used to enhance the rheological properties of asphalt binders and to improve the rutting resistance of the asphalt mixtures. Kim et al. [14] and Bernier et al. [15] studied the effect of the amount of recycled asphalt pavement materials on the antirutting performance of polymermodified asphalt. They observed that the incorporation of recycled asphalt pavement materials can improve the rutting resistance of the asphalt mixtures. Hydrated lime [16, 17], graphite [18], and steel slag [19, 20] have been mixed into the asphalt mixtures to partially replace the mineral filler or the asphalt mixture. Subsequently, the hightemperature performances of the corresponding modified mixtures were evaluated. The results indicated that such mixtures exhibit better rutting resistance than the control asphalt mixture. Coleri et al. observed that dense gradation and large aggregate size improve aggregate interlocking, which can effectively disperse the shear stress distribution within the asphalt pavement, improving the shear resistance and the hightemperature performance [21]. Shanbara et al. found that, compared with the conventional cold and hot mixtures, the cold mix asphalt reinforced with the natural and synthetic fibers shows better resisting permanent deformation damage [22, 23]. Reflective cool pavements can prevent the occurrence of urban heat islands as well as the occurrence of pavement rutting to a certain extent [24–27]. The aforementioned studies have undoubtedly helped improve the hightemperature rutting resistance of asphalt pavements by improving the hightemperature performance of the asphalt binder and asphalt mixtures or reducing the pavement temperature. However, they have rarely considered performing improvements by optimizing the asphalt pavement structure combination.
In China, the upper, middle, and lower layers of asphalt pavements have conventionally used aggregates in the order of fine, medium, and coarse, or in the order of fine, medium, and medium granular in asphalt mixtures. Furthermore, the asphalt mixture of each structural layer is designed to exhibit the complete range of functional requirements; i.e., each asphalt structural layer is designed to achieve good rutting resistance, cracking resistance, and moisture sensitivity. Researchers have observed that pavement rutting mainly appears in the middle layer of the asphalt pavement structure; therefore, the middlelayer mixtures must be designed to be the most resistant to rutting [28–30]. However, lowtemperature crack resistance and moisture sensitivity of the middlelayer mixtures are also considered during the asphalt mixture design; thus, maximizing the rutting resistance of the middle layer is impossible. Moreover, a previous study has proved that the lowerlayer mixtures mainly provide resistance to fatigue cracking in asphalt pavements; therefore, the lowerlayer mixtures should exhibit good crack resistance. However, these mixtures are typically designed to provide temperature stability and moisture sensitivity; therefore, the crack resistance of these mixtures is not maximized [31]. Therefore, it is significantly important to design the asphalt pavement structure according to the individual functional needs of each asphalt structural layer.
This study thereby intends to improve the typical semirigid base asphalt pavement structure with an inverted asphalt pavement structure (IAPS), wherein the middle and lower layers of the standard asphalt pavement are switched. Subsequently, the BISAR 3.0 software and a custombuilt ruttesting rig were used to test the resistance of 18 cm thick slab specimen. The test results offer significant improvements in the asphalt pavement structure design.
2. Inverted Asphalt Pavement Structure and Theoretical Verification
2.1. Inverted Asphalt Pavement Structure
Structural engineers have observed that, in threelayered asphalt pavements, ruts typically originate in the middle layer [28–30]. Theoretical studies have also denoted that the maximum shear stress of the semirigid base asphalt pavement gradually shifts downward with an increase in load pressure; however, this stress is always observed in the middle layer [32, 33]. Therefore, the middle layer of asphalt pavements should have sufficient hightemperature rutting resistance [32, 33]. The nominal maximum particle size of the aggregate significantly affects the hightemperature stability of an asphalt mixture. Large nominal particle sizes have been observed to improve the hightemperature rutting resistance of the asphalt mixture [34]. This observation inspired the IAPS, in which the bottom two layers of the pavement structure typically applied in China were switched. The properties of all the layers in both pavement structure types are presented in Table 1, where TAPS represents the traditional asphalt pavement structure.

2.2. Theoretical Verification of the Inverted Asphalt Pavement Structure
2.2.1. Calculation Parameter
Table 2 shows the parameter that is used for calculating the stress in different asphalt pavement structures. The moduli of the AC13, AC20, and AC25 asphalt mixtures were tested in the laboratory according to the Standard Test Methods of Bitumen and Bituminous Mixtures for Highway Engineering (JTG E202011) [35], and the test temperature was set to 20°C. The Poisson’s ratios of the monolithic materials, including the asphalt mixtures and the cementstabilized macadam base, and the bulk material (soil base) were observed to be 0.25 and 0.4, respectively.

2.2.2. Calculation Results
The stress distributions in the two asphalt pavement structures were calculated using the BISAR 3.0 software. The calculation results of the maximum shear stress in the two asphalt pavement structures are presented in Table 3, where and denote the maximum shear stress of the TAPS and IAPS, respectively. It is noteworthy that an asphalt pavement structure is considered to be a linear elastic layer system in these stress calculations, and the interlayer contact is modeled to be completely continuous.

Table 3 shows that the maximum shear stress of the IAPS is lower than that of the TAPS by 1.7%. This indicates that the IAPS can improve the hightemperature rutting resistance of the asphalt pavement.
3. Rutting Test Verification of the Inverted Asphalt Pavement Structure
3.1. Raw Materials and Mixtures
3.1.1. Asphalt Binder
The SBS (IC)modified asphalt, produced by Zhejiang Yinji Petrochemical Co. Ltd. (Zhejiang Province, China), was used as the binder for the AC13 asphalt mixture and as the gluing material between two asphalt layers. Class A70# matrix asphalt, produced by the Zhenhai Refining & Chemical Company (Zhejiang Province, China), was used as the binder for the AC20 and AC25 asphalt mixtures. The technical properties of the two asphalt binders are presented in Table 4.

3.1.2. Aggregate
Crushed basalt was used as the coarse aggregate for the AC13 asphalt mixture, whereas crushed limestone was used as the coarse aggregate for the AC20 and AC25 asphalt mixtures. The fine aggregate and mineral powder that were used for the AC13 and those for AC20 and AC25 asphalt mixtures were crushed limestone and limestone ore, respectively. The coarse aggregate, fine aggregate, and mineral powder were produced by the Jinhua Pan’an Stone Material Factory (Zhejiang Province, China), and each material satisfied the requirements mandated by the Technical Specification for Construction of Highway Asphalt Pavements (JTG F402004) [36].
3.1.3. Gradation
The aggregate gradations of the asphalt mixtures that are used in this study are presented in Table 5.

3.1.4. Mix Design
In this study, the AC13, AC20, and AC25 asphalt mixtures were designed using the Marshall design procedure. The mixture design and road performance test results of the AC13, AC20, and AC25 asphalt mixtures are presented in Tables 6 and 7, respectively, where VV, VMA, VFA, DS, , , and TSR denote the air void volume, voids in mineral aggregate, volume of voids ﬁlled with asphalt, dynamic stability, flexural tensile strain, retained Marshall stability, and freezethaw splitting strength ratio, respectively. VV, VMA, VFA, DS, , , and TSR were verified according to the Standard Test Methods of Bitumen and Bituminous Mixtures for Highway Engineering (JTG E202011) [35].


The results in Table 7 denote that the road performance indicators, such as DS, , , and TSR, of the asphalt mixtures used in this study satisfy the technical requirements of the Technical Specification for Construction of Highway Asphalt Pavements (JTG F402004) [36]. The dynamic stability of the AC25 asphalt mixture is notably higher than that of the AC20 asphalt mixture.
3.2. Test Method
3.2.1. Preparation of the 18 cm Thick Slab Specimen
Considering that the traditional slab specimen forming instrument can produce slab specimens with a thickness of 3–10 cm, the 18 cm thick slab specimen was prepared using a custombuilt slab specimen forming instrument. The main technical indexes and parameters of the custombuilt instrument are identical to those of the traditional instrument; however, the custombuilt instrument can produce slab specimens with a thickness of 3–20 cm.
To simulate the actual field conditions of the upper, middle, and lower asphalt layers, the slab specimen was prepared in the laboratory as follows:(1)The lowerlayer slab specimen: first, a 300 mm × 300 mm layer of board (see Figure 1) was produced using the custombuilt slab specimen forming instrument, satisfying the layerwise thickness requirement denoted in Table 1. When the lower layer was AC20 asphalt mixture, the thickness of the produced slab specimen was 6 cm; when AC25 asphalt mixture was used as the lower layer, the board thickness was 8 cm. Then, the slab specimens were placed at room temperature for at least 24 h. Subsequently, the SBSmodified asphalt weighing 0.4 L/m^{2} was evenly sprayed on the slab specimen surface and was cured for at least 2 h.(2)The middlelayer slab specimen: the middlelayer slab specimen was produced and applied on the lowerlayer slab specimen sprayed with the sticky layer oil, with thicknesses as specified in Table 1. When the AC20 asphalt mixture was used as the middle layer, the board thickness was 6 cm; when the AC25 asphalt mixture was used as the middle layer, its thickness was 8 cm. The SBSmodified asphalt weighing 0.4 L/m^{2} was evenly sprayed on the surface of the prepared middlelayer slab specimen, which was subsequently cooled at room temperature for 24 h.(3)The upperlayer slab specimen: finally, the 4 cm thick toplayer slab specimen was produced and applied on the middlelayer slab specimen sprayed with the sticky layer oil. Subsequently, it was cooled at room temperature for 48 h. The production process of the upperlayer slab specimen is depicted in Figure 2.
Each asphalt layer was produced with the optimal asphalt content and the mixture density specified in the Standard Test Methods of Bitumen and Bituminous Mixtures for Highway Engineering (JTG E202011) [35]. To ensure the reliability of the rutting tests, the porosity difference in all slab specimens was maintained within 1% from that of the respective standard cylindrical specimens [37]. The demolded 18 cm thick slab specimen is denoted in Figure 3.
3.2.2. Rutting Test
The rutting test was conducted on a custommade rutting tester for a thick slab specimen (18 cm thick). The main difference between the traditional rutting tester and the custommade rutting tester is that the former can be used only to test the rutting depth of the slab specimen with a height of 5–10 cm, whereas the custommade rutting tester can be used to measure the rutting depth of the slab specimen with a height of 5–20 cm. Other test procedures of the custommade and traditional rutting tester are identical. For the rutting test, the test temperature was 60°C, the loading rate was 42 times/min, the total testing time was 10 h, and the wheel loads were 0.7 and 1.2 MPa.
The Standard Test Methods of Bitumen and Bituminous Mixtures for Highway Engineering (JTG E202011) [35] specifies that the prepared slab specimen should be placed into a constanttemperature (60°C) oven before testing to ensure that the internal temperature of the slab specimen is equal to the temperature at which rutting occurs. Generally, when the slab specimen is 5–10 cm thick, the holding time of the slab specimen in a 60°C oven should be 5–12 h. However, the slab specimen investigated in this study is thicker than most other samples (at 18 cm), and we could find no reference data to indicate the duration for which thick slab specimens should be kept in the oven. If the holding time is too short, the internal temperature of the slab specimen will not reach the mandated test temperature; however, if the holding time is too long, the binder and mixtures will age, affecting the reliability of the test results. Therefore, the relationship between the holding time and the internal temperature of the 18 cm thick slab specimen was recorded in preliminary tests and is depicted in Figure 4. During the test, the temperature of the oven was maintained to be constant at 60°C. The internal temperatures between the upper and middle asphalt layers and those between the middle and lower asphalt layers were tested using temperature sensors that were embedded within the pavement layers during the slab specimen preparation. The temperature test procedure is shown in Figure 5.
As shown in Figure 4, when the holding time of a slab specimen is lower than 4 h, the internal temperatures of the 18 cm thick slab specimen increase sharply with increase in the holding time. When the holding time is 4 h, the internal temperatures of the slab specimen reach 55°C; furthermore, when the holding time is 8 h, the internal temperatures of the slab specimen are stable at ∼60°C, which is the temperature at which the loading tests are conducted. Therefore, to ensure that the internal temperatures of the slab specimen are equal to the mandated rutting test temperature, we suggest that the holding time of an 18 cm thick slab specimen should be kept in an oven at 60°C for 8 h.
4. Results and Discussion
4.1. Rutting Test Results
Figure 6 shows the laboratory rutting test process of the 18 cm thick slab specimen. Moreover, the rutting test results of slab specimens in different pavement structures are presented in Table 8.

As denoted by the results in Table 8, the cumulative rut depths of the two asphalt pavement structures under different wheel loads increase as the number of load cycles increases. Furthermore, the cumulative rut depths of the IAPS samples tend to be smaller than those of the TAPS when the load cycles and wheel loads are the same. Considering that the number of the testing samples is small, an analysis of variance test was conducted to examine the differences between the rut depths of two pavement structures [38, 39]. Tables 9 and 10 present the significant test results of the two pavement structures under wheel loads of 0.7 MPa and 1.2 MPa, respectively.
 
significant at . 
 
significant at . 
As presented in Tables 9 and 10, the differences between the rut depths of the TAPS and IAPS samples that are subjected to the same number of load cycles are significant. These findings show that the IAPS sample is more resistant against rutting than the TAPS sample.
4.2. RutDevelopment Trend and Prediction Equation
4.2.1. Development of Rut
According to the results presented in Table 8, the development trend of the cumulative rut depth of different pavement structures is plotted against the number of the loading cycles in Figure 7.
(a)
(b)
It can be seen from Figure 7 that the shapes of the rutdevelopment curves of both pavement structures are very similar when plotted against the increase of the number of loading cycles. When the number of loading cycles is less than 2550, the cumulative rut depths of both pavement structures increase sharply as the number of load cycles increases. However, after 2550 load cycles, the rate of increase in the cumulative rut depths of both structures decreases gradually until the rut depth stabilizes. The permanent deformation of asphalt mixture is mainly classified into three stages. During the first stage, the cumulative rut depths increase sharply as the number of load cycles increases. During the second stage, the rate of increase of the cumulative rut depths decreases gradually and eventually stabilizes. In the third stage, the strain rate grows rapidly with the increases of loading cycles. The material structure loses its stability under shear and finally results in the failure of the material [40]. Thus, Figure 7 only shows the first and second stage of the permanent deformation of asphalt mixture during the rutting experiment.
4.2.2. Rutting Prediction Equation
The rutdevelopment stages of asphalt pavement structures, as shown in Figure 7, indicate that there exists a horizontal asymptotic line during the second stage of permanent deformation of slab specimen in the rutdevelopment curve. Furthermore, the corresponding value of the asymptote during the second stage of permanent deformation can be interpreted as the maximum rut depth . We assume that the development of ruts during the first and second stages in asphalt pavement structures follows a rutting prediction equation, which should satisfy the following two boundary conditions: when , and when , ,
Where N denotes the number of loading cycles, denotes the rut depth (mm) of the slab specimen before any loading has been applied, and denotes the rut depth (mm) of the slab specimen at the number of final loading cycles of the second stage.
Furthermore, we fitted the resulting curves to establish the following equation according to the aforementioned boundary conditions:where denotes the rut depth (mm) of slab specimen after N loading cycles and and are the regression coefficients.
Equation (1) was used to fit the data presented in Table 8, and the resulting values of the coefficients , , and R^{2} are presented in Table 11.

Table 11 shows that the correlation coefficients R^{2} of the rutting prediction equation are greater than 0.98, indicating that the rutting prediction equation proposed in this study can accurately predict the development trend of rutting in the asphalt pavement structures.
4.3. Factors Influencing the Rutting Test
4.3.1. Effect of Wheel Load on Pavement Rutting
According to the values presented in Table 11, the effect of the wheel load on the maximum rut depth of the asphalt pavement structure is denoted in Table 12, where denotes the ratio of the maximum rut depth of the slab specimen under the wheel load of 1.2 MPa to that under the wheel load of 0.7 MPa.

As shown in Table 12, when the wheel load is increased from 0.7 MPa to 1.2 MPa, the rut depths of the different pavement structures increase by 63% or 72% depending on the pavement layer structure.
4.3.2. Effect of the Pavement Structure on Pavement Rutting
Based on the values presented in Table 11, the effect of the type of pavement structure with the same wheel loads on the maximum rut depth is shown in Table 13, where and denote the maximum rut depths of the IAPS and TAPS, respectively. Furthermore, denotes the ratio of the maximum rut depth of the IAPS to that of the TAPS under the same wheel load.

As shown in Table 13, the IAPS sample contained ruts that were 16% and 12% shallower than those in the TAPS sample under the same wheel loads of 0.7 MPa and 1.2 MPa, respectively.
5. Conclusions
An inverted asphalt pavement structure was proposed in this study, and the rutting resistance of the inverted asphalt pavement structure was evaluated. The following conclusions can be obtained from the abovementioned results.(1)When compared with the TAPS, the maximum shear stress of the IAPS can be reduced by approximately 1.7%. These results show that the IAPS can reduce the maximum shear stress of asphalt pavements.(2)Two rutting prediction equations of asphalt pavement structures were established, and the correlation coefficients R^{2} exceeded 0.98. This high R^{2} value indicates that the proposed rutting prediction equation can accurately predict the rut development in asphalt pavements.(3)When compared with the TAPS, the rutting resistance of the IAPS under the wheel load of 0.7 MPa and 1.2 MPa can be increased by 16% and 12%, respectively. Furthermore, the increase in wheel load affects the rutting performances of both pavement structures in a similar manner. When the wheel load is increased from 0.7 MPa to 1.2 MPa, the rut depths of the different pavement structures increase by 63% or 72% depending on the pavement layer structure.
The aforementioned tests compared the rutting resistance of the TAPS and IAPS with different numbers of load cycles (≤25500). The effect of more load cycles will be observed in our future studies to further verify the reliability of the proposed rutting prediction equations and the superiority of the IAPS. Moreover, the paper primarily focused on the rutting resistance of the IAPS; the fatigue property of the IAPS also will be studied in our further work.
Data Availability
The data used to support the findings of this study are included within the article.
Conflicts of Interest
The authors declare that there are no conflicts of interest regarding the publication of this paper.
Acknowledgments
The research was supported by the Science and Technology Project of Zhejiang Provincial Department of Transportation (No. 2016020), the Science and Technology Project of Henan Provincial Department of Transportation (No. 2020J22), and the Scientific Research of Central Colleges of China for Chang’an University (No. 300102218212). The authors gratefully acknowledge these financial supports.
References
 V. D. Jarnette, L. M. McCarthy, T. Bennert, and M. C. Guercio, “Use of mechanisticempirical pavement design principles to assign asphalt pavement pay factor adjustments,” Journal of Construction Engineering and Management, vol. 139, no. 11, Article ID 04013024, 2013. View at: Publisher Site  Google Scholar
 M. Zheng, L. Han, F. Wang, H. Mi, Y. Li, and L. He, “Comparison and analysis on heat reflective coating for asphalt pavement based on cooling effect and antiskid performance,” Construction and Building Materials, vol. 93, pp. 1197–1205, 2015. View at: Publisher Site  Google Scholar
 W. S. Mogawer, A. J. Austerman, J. S. Daniel, F. J. Zhou, and T. Bennert, “Evaluation of the effects of hot mix asphalt density on mixture fatigue performance, rutting performance and MEPDG distress predictions,” International Journal of Pavement Engineering, vol. 12, no. 2, pp. 161–175, 2011. View at: Publisher Site  Google Scholar
 R. Gogoi, A. Das, and P. Chakroborty, “Are fatigue and rutting distress modes related?” International Journal of Pavement Research and Technology, vol. 6, no. 4, pp. 269–273, 2013. View at: Publisher Site  Google Scholar
 Y. F. Du, J. Q. Chen, Z. Han, and W. Z. Liu, “A review on solutions for improving rutting resistance of asphalt pavement and test methods,” Construction and Building Materials, vol. 168, pp. 893–905, 2018. View at: Publisher Site  Google Scholar
 A. I. AlHadidy and Y. Q. Tan, “Effect of styrenebutadienestyrene on the properties of asphalt and stonematrixasphalt mixture,” Journal of Materials in Civil Engineering, vol. 23, no. 4, pp. 504–510, 2011. View at: Publisher Site  Google Scholar
 V. O. Bulatovic, V. Rek, and K. J. Marković, “Rheological properties and stability of ethylene vinyl acetate polymermodified bitumen,” Polymer Engineering and Science, vol. 53, no. 11, pp. 2276–2283, 2013. View at: Publisher Site  Google Scholar
 H. Y. Yin, Y. G. Zhang, Y. F. Sun et al., “Performance of hot mix epoxy asphalt binder and its concrete,” Materials and Structures, vol. 48, no. 11, pp. 3825–3835, 2015. View at: Publisher Site  Google Scholar
 G. L. Zou and C. Wu, “Evaluation of rheological properties and field applications of buton rock asphalt,” Journal of Testing and Evaluation, vol. 43, no. 5, pp. 1146–1156, 2015. View at: Publisher Site  Google Scholar
 C. Q. Fang, X. Yu, R. E. Yu, P. Liu, and X. T. Qiao, “Preparation and properties of isocyanate and nano particles composite modified asphalt,” Construction and Building Materials, vol. 119, pp. 113–118, 2016. View at: Publisher Site  Google Scholar
 H. Geng, C. S. Clopotel, and H. U. Bahia, “Effects of high modulus asphalt binders on performance of typical asphalt pavement structures,” Construction and Building Materials, vol. 44, pp. 207–213, 2013. View at: Publisher Site  Google Scholar
 P. Hajikarimi, M. Rahi, and F. M. Nejad, “Comparing different rutting specification parameters using high temperature characteristics of rubbermodified asphalt binders,” Road Materials and Pavement Design, vol. 16, no. 4, pp. 751–766, 2015. View at: Publisher Site  Google Scholar
 Z. J. Dong, G. Q. Xiao, and X. B. Gong, “Analysis on impact of gradation and antirutting additive on rutting resistance of asphalt mixture,” Journal of Highway and Transportation Research and Development, vol. 31, no. 2, pp. 27–31, 2014. View at: Google Scholar
 S. Kim, G. A. Sholar, T. Byron, and J. Kim, “Performance of polymermodified asphalt mixture with reclaimed asphalt pavement,” Transportation Research Record, vol. 2126, no. 2126, pp. 109–114, 2009. View at: Publisher Site  Google Scholar
 A. Bernier, A. Zofka, and I. Yut, “Laboratory evaluation of rutting susceptibility of polymermodified asphalt mixtures containing recycled pavements,” Construction and Building Materials, vol. 31, pp. 58–66, 2012. View at: Publisher Site  Google Scholar
 M. Nazirizad, A. Kavussi, and A. Abdi, “Evaluation of the effects of antistripping agents on the performance of asphalt mixtures,” Construction and Building Materials, vol. 84, pp. 348–353, 2015. View at: Publisher Site  Google Scholar
 A. K. Das and D. Singh, “Investigation of rutting, fracture and thermal cracking behavior of asphalt mastic containing basalt and hydrated lime fillers,” Construction and Building Materials, vol. 141, pp. 442–452, 2017. View at: Publisher Site  Google Scholar
 Z. G. Wang, Q. L. Dai, and S. C. Guo, “Laboratory performance evaluation of both flake graphite and exfoliated graphite nanoplatelet modified asphalt composites,” Construction and Building Materials, vol. 149, pp. 515–524, 2017. View at: Publisher Site  Google Scholar
 S. P. Wu, Y. J. Xue, Q. S. Ye, and Y. C. Chen, “Utilization of steel slag as aggregates for stone mastic asphalt (SMA) mixtures,” Building and Environment, vol. 42, no. 7, pp. 2580–2585, 2007. View at: Publisher Site  Google Scholar
 E. A. Oluwasola, M. R. Hainin, and M. M. A. Aziz, “Comparative evaluation of densegraded and gapgraded asphalt mix incorporating electric arc furnace steel slag and copper mine tailings,” Journal of Cleaner Production, vol. 122, pp. 315–325, 2016. View at: Publisher Site  Google Scholar
 E. Coleri, J. T. Harvey, K. Yang, and J. M. Boone, “Investigation of asphalt concrete rutting mechanisms by Xray computed tomography imaging and micromechanical finite element modeling,” Materials and Structures, vol. 46, no. 6, pp. 1027–1043, 2013. View at: Publisher Site  Google Scholar
 H. K. Shanbara, F. Ruddock, and W. Atherton, “A viscoplastic model for permanent deformation prediction of reinforced cold mix asphalt,” Construction and Building Materials, vol. 186, pp. 287–302, 2018. View at: Publisher Site  Google Scholar
 H. K. Shanbara, A. Shubbar, F. Ruddock, and W. Atherton, “Characterizing the rutting behaviour of reinforced cold mix asphalt with natural and synthetic fibres using finite element analysis,” in Advances in Structural Engineering and Rehabilitation, pp. 221–227, Springer Nature, Singapore, 2020. View at: Publisher Site  Google Scholar
 M. Santamouris, “Using cool pavements as a mitigation strategy to fight urban heat island—a review of the actual developments,” Renewable and Sustainable Energy Reviews, vol. 26, no. 10, pp. 224–240, 2013. View at: Publisher Site  Google Scholar
 Y. J. Jiang, C. Q. Deng, Z. J. Chen, and Y. H. Tian, “Evaluation of the cooling effect and antirutting performance of thermally resistant and heatreflective pavement,” International Journal of Pavement Engineering, vol. 21, no. 4, pp. 447–456, 2020. View at: Publisher Site  Google Scholar
 Y. J. Jiang, Y. Q. Ye, J. S. Xue, and Z. J. Chen, “Thermal resistant stone mastic asphalt surface and its antirutting performance,” Journal of Materials in Civil Engineering, vol. 30, no. 11, Article ID 06018019, 2018. View at: Publisher Site  Google Scholar
 T. Ma, Y. Zhong, T. Tang, and X. M. Huang, “Design and evaluation of heatresistant asphalt mixture for permafrost regions,” International Journal of Civil Engineering, vol. 14, no. 5, pp. 339–346, 2016. View at: Publisher Site  Google Scholar
 T. Xu and X. M. Huang, “Investigation into causes of inplace rutting in asphalt pavement,” Construction and Building Materials, vol. 28, no. 1, pp. 525–530, 2012. View at: Publisher Site  Google Scholar
 H. Wang, Q. S. Zhang, and J. Q. Tan, “Investigation of layer contributions to asphalt pavement rutting,” Journal of Materials in Civil Engineering, vol. 21, no. 4, pp. 181–185, 2009. View at: Publisher Site  Google Scholar
 J. Yang, L. M. Yu, J. Wang, J. Chen, and G. C. Qian, “Rutting resistance of asphalt mixtures in the middle course,” Journal of Southeast University (English Edition), vol. 22, no. 2, pp. 270–272, 2006. View at: Google Scholar
 Z. Z. Li, S. F. Chen, W. D. Liao, and H. X. Chen, “Evaluation of anticracking performance of modified HMA in stress absorbing layers under low temperature,” China Journal of Highway and Transport, vol. 25, no. 4, pp. 29–35, 2012, in Chinese. View at: Google Scholar
 Q. Li, H. H. Yang, F. J. Ni, X. Ma, and L. H. Luo, “Cause analysis on permanent deformation for asphalt pavements using field cores,” Construction and Building Materials, vol. 100, pp. 40–51, 2015. View at: Publisher Site  Google Scholar
 Y. Zhang, X. Luo, Y. Deng, S. G. Hou, X. J. Shi, and R. L. Lytton, “Evaluation of rutting potential of flexible pavement structures using energybased pseudo variables,” Construction and Building Materials, vol. 247, Article ID 118391, 2020. View at: Publisher Site  Google Scholar
 D. Han, L. Wei, and J. Zhang, “Experimental study on performance of asphalt mixture designed by different method,” Procedia Engineering, vol. 137, pp. 407–414, 2016. View at: Publisher Site  Google Scholar
 Ministry of Transport of the People’s Republic of China, Standard Test Methods of Bitumen and Bituminous Mixtures for Highway Engineering (JTG E202011), China Communications Press, Beijing, China, 2011, in Chinese.
 Ministry of Transport of the People’s Republic of China, Technical Speciﬁcations for Construction of Highway Asphalt Pavements (JTG F402004), China Communications Press, Beijing, China, 2004, in Chinese.
 Y. J. Jiang, C. Q. Deng, J. S. Xue, and Z. J. Chen, “Investigation into the performance of asphalt mixture designed using different methods,” Construction and Building Materials, vol. 177, pp. 378–387, 2018. View at: Publisher Site  Google Scholar
 Y. J. Jiang, C. Q. Deng, Q. Li, and H. P. Liu, “Effect of compaction methods on physical and mechanical properties of asphalt mixture,” Journal of Materials in Civil Engineering, vol. 31, no. 6, Article ID 04019075, 2019. View at: Publisher Site  Google Scholar
 Y. J. Jiang, C. Q. Deng, J. S. Xue, H. P. Liu, and Z. J. Chen, “Investigation of the fatigue properties of asphalt mixture designed using vertical vibration method,” Road Materials and Pavement Design, vol. 21, no. 5, pp. 1454–1469, 2020. View at: Publisher Site  Google Scholar
 S. G. Hou, X. J. Shi, Y. Deng, and F. Gu, “Evaluation of rutting and friction resistance of hot mix asphalt concrete using an innovative vertically loaded wheel tester,” Construction and Building Materials, vol. 176, pp. 710–719, 2018. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2020 Yingjun Jiang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.